Lecture Notes: BCS Theory of Superconductivity
Total Page：16
File Type：pdf, Size：1020Kb
Lecture Notes: BCS theory of superconductivity Prof. Rafael M. Fernandes Here we will discuss a new ground state of the interacting electron gas: the superconducting state. In this macroscopic quantum state, the electrons form coherent bound states called Cooper pairs, which dramatically change the macroscopic properties of the system, giving rise to perfect conductivity and perfect diamagnetism. We will mostly focus on conventional superconductors, where the Cooper pairs originate from a small attractive electron-electron interaction mediated by phonons. However, in the so- called unconventional superconductors - a topic of intense research in current solid state physics - the pairing can originate even from purely repulsive interactions. 1 Phenomenology Superconductivity was discovered by Kamerlingh-Onnes in 1911, when he was studying the transport properties of Hg (mercury) at low temperatures. He found that below the liquifying temperature of helium, at around 4:2 K, the resistivity of Hg would suddenly drop to zero. Although at the time there was not a well established model for the low-temperature behavior of transport in metals, the result was quite surprising, as the expectations were that the resistivity would either go to zero or diverge at T = 0, but not vanish at a ﬁnite temperature. In a metal the resistivity at low temperatures has a constant contribution from impurity scattering, a T 2 contribution from electron-electron scattering, and a T 5 contribution from phonon scattering. Thus, the vanishing of the resistivity at low temperatures is a clear indication of a new ground state. Another key property of the superconductor was discovered in 1933 by Meissner. He found that the magnetic ﬂux density B is expelled below the superconducting transition temperature Tc, i.e. B = 0 inside a superconductor material - the so-called Meissner eﬀect. This means that the superconductor is a perfect diamagnet. Recall that the relationship between B, the magnetic ﬁeld H, and the magnetization M is given by: B = H + 4πM (1) Therefore, since B = 0 for a superconductor, the magnetic susceptibility χ = @M=@H is given by: 1 χ = − (2) 4π If one increases the magnetic ﬁeld applied to a superconductor, it eventually destroys the superconduct- ing state, driving the system back to the normal state. In type I superconductors, there is no intermediate 1 state separating the transition from the superconducting to the normal state upon increasing ﬁeld. In type II superconductors, on the other hand, there is an intermediate state, called mixed state, which appears before the transition to the normal state. In the mixed state, the magnetic ﬁeld partially penetrates the material via the formation of an array of ﬂux tubes carrying a multiple of the magnetic ﬂux quantum hc Φ0 = 2jej . The ﬁrst question we want to address is: which one of these two properties is “more fundamental”, perfect conductivity or perfect diamagnetism? Let us study the implications of perfect conductivity using Maxwell equations. If a material is a perfect conductor, application of a an electric ﬁeld freely accelerates the electric charge: m¨r = −eE (3) But since the current density is given by J = −ensr_ , where ns is the number of “superconducting electrons”, we have: n e2 J_ = s E (4) m From Faraday law, we have: 1 @B r × E = − (5) c @t which implies: @J n e2 @B r × = − s (6) @t cm @t But Ampere law gives 4π r × B = J (7) c and we obtain: @B 4πn e2 @B r × r × = − s (8) @t mc2 @t Using the identity r × r × C = r (r · C) − r2C and Maxwell equation r · B = 0, we obtain the equation: @B @B r2 = λ−2 (9) @t @t 2 where we deﬁned the penetration depth: s mc2 λ = 2 (10) 4πnse What is the meaning of Eq. (9)? Consider a one-dimensional system that is a perfect conductor for x > 0. Solving the diﬀerential equation for x, and taking into account the boundary conditions, we obtain that the derivative @B=@t decays exponentially with x, i.e. @B @B = e−x/λ (11) @t @t x=0 This means that the magnetic ﬁeld inside a perfect conductor is constant over time. However, this is not the Meissner eﬀect, which implies that the magnetic ﬁeld is zero - not a constant - inside the superconductor. For instance, consider that a magnetic ﬁeld B0 is applied to the material above Tc, when it is not yet a superconductor. If we cool down the system below Tc, the Meissner eﬀect says that B0 has to be expelled from the material, since B = 0 inside it. However, for a perfect conductor the ﬁeld would remain B0 inside the material. This exercise tells us that a superconductor is not just a perfect conductor! Based on this fact, the London brothers proposed a phenomenological model to describe the supercon- ductors that arbitrarily eliminates the time derivatives from Eq. (9): r2B = λ−2B (12) This equation correctly captures the Meissner eﬀect, as we discussed above, emphasizing the perfect diamagnetic properties of the superconductor. Combined with Ampere law, this equation implies the following relationship between J and B: n e2 r × J = − s B (13) mc Since B = r × A, where A is the magnetic vector potential, the equation above becomes the London equation n e2 J = − s A (14) mc in the so-called Coulomb gauge r · A = 0, i.e. in the gauge where the vector potential has only a non-zero transverse component. This gauge must be chosen because, from the continuity equation, the identity r · J = 0 must be satisﬁed. How can we justify London equation? From a phenomenological point of view, it follows from the rigidity of the wave-function in the superconducting state. For instance, according to Bloch theorem, the total momentum of the system in its ground state (i.e. in the absence of any applied ﬁeld) has a zero average value, hΨ jpj Ψi = 0. Now, let us assume that the wave-function Ψ is rigid, i.e. that this 3 relationship holds even in the presence of an external ﬁeld. Then, since the canonical momentum is given by p = mv − eA=c, we obtain: eA hvi = (15) mc Since J = −ens hvi, we recover London equation (14). Of course, the main question is about the microscopic mechanism that gives rise to this wave-function rigidity and, ultimately, to the superconducting state. Several of the most brilliant physicists of the last century tried to address this question - such as Bohr, Einstein, Feynman, Born, Heisenberg - but the answer only came in 1957 with the famous theory of Bardeen, Cooper, and Schrieﬀer (BCS) - almost 50 years after the experimental discovery by Kamerlingh-Onnes! Key experimental contributions made the main properties of the superconductors more transparent before the BCS theory appeared in 1957. The observation of an exponential decay of the speciﬁc heat at low temperatures showed that the energy spectrum of a superconductor is gapped. This is in contrast to the spectrum of a regular metal, which is gapless - recall that exciting an electron-hole pair near the Fermi surface costs very little energy to the metal. Another key experiment was the observation of the isotope eﬀect. By studying the superconducting transition temperature Tc of materials containing a diﬀerent element isotope, it was shown that Tc decays with M −1=2, where M is the mass of the isotope. Since this mass is related only to the ions forming the lattice, this experimental observation indicated that the lattice - and therefore the phonons - must play a key role in the formation of the superconducting state. The main point of the BCS theory is that the attractive electron-electron interaction mediated by the phonons gives rise to Cooper pairs, i.e. bound states formed by two electrons of opposite spins and momenta. These Cooper pairs form then a coherent macroscopic ground state, which displays a gapped spectrum and perfect diamagnetism. Key to the formation of Cooper pairs is the existence of a well-deﬁned Fermi surface, as we will discuss below. 2 One Cooper pair Much of the physics involved in the BCS theory can be discussed in the context of a simple quantum mechanics problem. Consider two electrons that interact with each other via an attractive potential V (r1 − r2). The Schrödinger equation is given by: 2 2 2 2 ~ rr ~ rr − 1 − 2 + V (r − r ) Ψ(r ; r ) = EΨ(r ; r ) (16) 2m 2m 1 2 1 2 1 2 where Ψ(r1; r2) is the wave-function and E, the energy. As usual, we change variables to the relative 1 displacement r = r1 − r2 and to the position of the center of mass R = 2 (r1 + r2). In terms of these new 4 variables, the Schrödinger equation becomes: 2r2 2r2 −~ R − ~ r + V (r) Ψ(r; R) = EΨ(r; R) (17) 2m∗ 2µ where m∗ = 2m is the total mass and µ = m=2 is the reduced mass. Since the potential does not depend on the center of mass coordinate R, we look for the solution: Ψ(r; R) = (r) eiK·R (18) which gives: 2r2 −~ r + V (r) (r) = E~ (r) (19) 2µ 2 2 ~ ~ K ~ where we deﬁned E = E − 2m∗ . For a given eigenvalue E, the lowest energy E is the one for which K = 0, i.e. for which the momentum of the center of mass vanishes. Thus, for now we consider E = E~. In this case, the two electrons have opposite momenta. Depending on the symmetry of the spatial part of the wave-function, even (r) = (−r) or odd (r) = − (−r), the spins of the electrons will form either a singlet or a triplet state, respectively, in order to ensure the anti-symmetry of the total wave-function.